LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: r56321, T = 450 C, P = 13.4 kbar, cell volume = 192.24 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003270
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56321, T = 450 C, P = 13.4 kbar, cell volume = 192.24 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7714
_cell_length_b                   5.7714
_cell_length_c                   5.7714
_cell_volume                     192.240
_cell_formula_units_Z            4
_database_code_amcsd             0003359
_diffrn_ambient_pressure         1.34e+06
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    2.131
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003270
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56409, T = 450 C, P = 22.8 kbar, cell volume = 185.29 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003271
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56409, T = 450 C, P = 22.8 kbar, cell volume = 185.29 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7010
_cell_length_b                   5.7010
_cell_length_c                   5.7010
_cell_volume                     185.290
_cell_formula_units_Z            4
_database_code_amcsd             0003360
_diffrn_ambient_pressure         2.28e+06
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    2.210
_cod_original_cell_volume        185.291
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003271
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: als9k20, T = 500 C, P = 0.0 kbar, cell volume = 207.78 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003272
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als9k20, T = 500 C, P = 0.0 kbar, cell volume = 207.78 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9229
_cell_length_b                   5.9229
_cell_length_c                   5.9229
_cell_volume                     207.780
_cell_formula_units_Z            4
_database_code_amcsd             0003361
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.971
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003272
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56317, T = 500 C, P = 14.2 kbar, cell volume = 192.69 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003273
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56317, T = 500 C, P = 14.2 kbar, cell volume = 192.69 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7759
_cell_length_b                   5.7759
_cell_length_c                   5.7759
_cell_volume                     192.690
_cell_formula_units_Z            4
_database_code_amcsd             0003362
_diffrn_ambient_pressure         1.42e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.126
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003273
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r53621, T = 500 C, P = 15.8 kbar, cell volume = 191.35 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003274
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53621, T = 500 C, P = 15.8 kbar, cell volume = 191.35 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7625
_cell_length_b                   5.7625
_cell_length_c                   5.7625
_cell_volume                     191.352
_cell_formula_units_Z            4
_database_code_amcsd             0003363
_diffrn_ambient_pressure         1.58e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.140
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003274
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56405, T = 500 C, P = 23.6 kbar, cell volume = 185.62 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003275
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56405, T = 500 C, P = 23.6 kbar, cell volume = 185.62 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7044
_cell_length_b                   5.7044
_cell_length_c                   5.7044
_cell_volume                     185.622
_cell_formula_units_Z            4
_database_code_amcsd             0003364
_diffrn_ambient_pressure         2.36e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.207
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003275
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: als8k20, T = 550 C, P = 0.0 kbar, cell volume = 210.08 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003276
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als8k20, T = 550 C, P = 0.0 kbar, cell volume = 210.08 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9447
_cell_length_b                   5.9447
_cell_length_c                   5.9447
_cell_volume                     210.082
_cell_formula_units_Z            4
_database_code_amcsd             0003365
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    1.950
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003276
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56313, T = 550 C, P = 15.0 kbar, cell volume = 193.05 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003277
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56313, T = 550 C, P = 15.0 kbar, cell volume = 193.05 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7795
_cell_length_b                   5.7795
_cell_length_c                   5.7795
_cell_volume                     193.050
_cell_formula_units_Z            4
_database_code_amcsd             0003366
_diffrn_ambient_pressure         1.5e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.122
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003277
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r53693, T = 550 C, P = 17.6 kbar, cell volume = 190.27 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003278
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r53693, T = 550 C, P = 17.6 kbar, cell volume = 190.27 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7516
_cell_length_b                   5.7516
_cell_length_c                   5.7516
_cell_volume                     190.268
_cell_formula_units_Z            4
_database_code_amcsd             0003367
_diffrn_ambient_pressure         1.76e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.153
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003278
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56401, T = 550 C, P = 24.5 kbar, cell volume = 185.89 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003279
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56401, T = 550 C, P = 24.5 kbar, cell volume = 185.89 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7071
_cell_length_b                   5.7071
_cell_length_c                   5.7071
_cell_volume                     185.886
_cell_formula_units_Z            4
_database_code_amcsd             0003368
_diffrn_ambient_pressure         2.45e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.203
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003279
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56429, T = 550 C, P = 25.1 kbar, cell volume = 185.10 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003280
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56429, T = 550 C, P = 25.1 kbar, cell volume = 185.10 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.6990
_cell_length_b                   5.6990
_cell_length_c                   5.6990
_cell_volume                     185.096
_cell_formula_units_Z            4
_database_code_amcsd             0003369
_diffrn_ambient_pressure         2.51e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.213
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003280
Halite-sylvite thermoelasticity Sample: r56437, T = 550 C, P = 25.1 kbar, cell volume = 185.11 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003281
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56437, T = 550 C, P = 25.1 kbar, cell volume = 185.11 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.6991
_cell_length_b                   5.6991
_cell_length_c                   5.6991
_cell_volume                     185.105
_cell_formula_units_Z            4
_database_code_amcsd             0003370
_diffrn_ambient_pressure         2.51e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.213
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003281
Halite-sylvite thermoelasticity Sample: r56453, T = 550 C, P = 25.2 kbar, cell volume = 185.51 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003282
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56453, T = 550 C, P = 25.2 kbar, cell volume = 185.51 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7033
_cell_length_b                   5.7033
_cell_length_c                   5.7033
_cell_volume                     185.515
_cell_formula_units_Z            4
_database_code_amcsd             0003371
_diffrn_ambient_pressure         2.52e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.208
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003282
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: als7k20, T = 600 C, P = 0.0 kbar, cell volume = 212.03 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003283
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als7k20, T = 600 C, P = 0.0 kbar, cell volume = 212.03 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.9630
_cell_length_b                   5.9630
_cell_length_c                   5.9630
_cell_volume                     212.029
_cell_formula_units_Z            4
_database_code_amcsd             0003372
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.932
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003283
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56309, T = 600 C, P = 15.8 kbar, cell volume = 193.46 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003284
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56309, T = 600 C, P = 15.8 kbar, cell volume = 193.46 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7836
_cell_length_b                   5.7836
_cell_length_c                   5.7836
_cell_volume                     193.462
_cell_formula_units_Z            4
_database_code_amcsd             0003373
_diffrn_ambient_pressure         1.58e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.117
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003284
_amcsd_formula_title             (K.2Na.8)Cl
Halite-sylvite thermoelasticity Sample: r56281, T = 600 C, P = 17.4 kbar, cell volume = 191.66 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003285
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r56281, T = 600 C, P = 17.4 kbar, cell volume = 191.66 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.2Na.8)Cl
_chemical_formula_sum            'Cl K0.2 Na0.8'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.7656
_cell_length_b                   5.7656
_cell_length_c                   5.7656
_cell_volume                     191.661
_cell_formula_units_Z            4
_database_code_amcsd             0003374
_diffrn_ambient_pressure         1.74e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.137
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.2 Na.8) Cl'
_cod_database_code               9003285
_amcsd_formula_title             (K.2Na.8)Cl